- Research
- Open Access

# Boltzmann equations and ab initio calculations: comparative study of cubic and wurtzite CdSe

- A. Abbassi
^{1}Email author, - Z. Zarhri
^{1}, - Ch. Azahaf
^{1}, - H. Ez-Zahraouy
^{1}and - A. Benyoussef
^{1}

**Received:**6 May 2015**Accepted:**7 September 2015**Published:**24 September 2015

## Abstract

The electronic and optical properties of CdSe in two phases, cubic and wurtzite, have been studied by first principal calculations using the density functional theory. The optical parameters such as transmittance, optical absorption, refractive index and extinction coefficient have been investigated. We have calculated also the band structure, and total/partial density of state using the full potential-linearized augmented plane wave method with the local density approximation, generalized gradient approximation and the modified Becke–Johnson functional (mBJ), implemented in the Wien2k package. With the mBJ approximation the gap found for cubic and wurtzite structure is direct and is equal to 1.85 and 1.7 eV respectively, what corresponds to the experiment results. The optical absorption is significant in the ultraviolet field while it becomes low beyond 600 nm in the visible light for CdSe in different structures. From λ = 400 nm the transmittance is stable and reaches 80 %. With Boltztrap package, we have investigated also that with increasing temperature, the electrical conductivity increases. During the calculation, the cubic structure has presented an isotropy. While for wurtzite CdSe, the propagation of waves into system is different in xx and zz directions. These results can be exploited in several applications of CdSe in optoelectronic devices.

## Keywords

- DFT
- Optical properties
- CdSe
- Wien2K
- Boltzmann
- Transmittance
- Optical absorption
- Band structure
- Optoelectronic

## Background

The semiconductor CdSe is type II–VI, consisting of an element of column II in the periodic table and an element from column VI. The cadmium atom is type II, it has two electrons in the valence band in orbital s, cd (4d10 5s2). The Selenium atom is material of type VI, it has six valence electrons in the s and p orbitals: 3d104s24p4. The valence band of the massive CdSe crystal consists essentially of the selenium p orbitals and the conduction band, of the cadmium orbital s. The massive CdSe material exists in two structures, cubic and wurtzite. The unit cell of Cd and Se is a hexagonal packing. The other form is the cubic structure, where the unit cell is cubic face-centered.

This type of semiconductors is considered an excellent candidate in optical devices technology, optical memories with high-density, transparent conductors, laser devices (Klude et al. 2002), photodetectors (Matsumura et al. 2002; Uthana and Reddy 1981) photoelectric sensors (Fuentes-Hernandez et al. 2004), solar cells (Merad et al. 2005; Merad et al. 2006; Karl and Jr 1982; Murray et al. 1993). It can be also used as a biological labeling (Jr et al. 1998), and in spintronic devices (Beaulac et al. 2008). The CdSe is transparent in infrared radiation, it is used sometimes in the fabrication of photoresistors and in thin layers for instruments using infrared light. This material is also highly luminescent.

CdSe crystallizes in two structures.

A hexagonal one, with space group P63 mc and the lattice parameters a = b = 4.299 A° and c = 7.010 A°. A cubic one, with space group F-43m and a = b = c 6.05 A°.

Several studies and research were treated CdSe using WIEN2k, treating its electronic properties, gap band (Akinci et al. 2009). The aim of this work is to investigate the electronic (DOS, PDOS, band structure), optical (absorption, transmittance, extinction factor, refractive index) and electrical (electrical conductivity) properties in both, CdSe Cubic and wurtzite phases. We will show that we can use CdSe in several applications of opto-electronic and photovoltaic.

This study is also a comparison between the two phases, we will demonstrate that our results obtained with this approximation mbj are in agreement with the experimental data.

## Calculation method

The present calculation is based on ab initio electronic structure. The first principles DFT calculations have been made with the full potential linearized augmented plane wave (FP LAPW) method using the WIEN2k program (Blaha et al. 2011). We also have to mention that our calculations have been performed using different approximations GGA (Perdew et al. 1996), LDA (Slater 1951) and modified Becke- Johnson functional (Blaha and Schwarz 2006).

In order to define the calculation of wave function, we used an energy cutoff of −8.0 Ryd for the LAPW. In this calculation we work with the 500 K-point and the self-consistent was found stable and converge at 10^{−6} Ryd.

We have noticed that α and β are the tensor indices, *ɛ*
_{
i,k
} is the band structure. N denotes the number of k-points that are sampled in the BZ.

## Electronic properties

### Band structure, total and partial DOS

In the hexagonal structure, the valence band is formed of an intense region from −3.89 to 0 eV essentially due to the orbital p of Se and a region from −8.04 to −7.04 eV which is mainly due to the orbital d of Cd. Beyond 1.7 eV, the conduction band is formed with a low occurrence of orbital d of Cd and p, d of Se.

It is also noted that the difference between the gap energy of wurtzite and cubic structure is ΔEg = 0.15 eV.

### Optical and transport properties

CdSe in wurtzite structure is not completely isotropic, the propagation of radiation in the direction xx and zz is different, especially in the range of 200–300 nm. The variation of the absorption in the region of ultraviolet and visible light of Wurtzite does not present a large difference with the cubic structure.

In the ultraviolet field, the transmittance is not stable and shows the lowest value for the cubic structure at λ = 144 nm where the reached value amounts 40 %. CdSe in its structure behaves as transparent in the visible light and absorbent in ultraviolet. These optical properties can be exploited in various optical applications.

The refractive index is also one of the optical properties of the systems, it describes the behavior of radiation propagating in materials. We have noted that in the absorbent systems, the refractive index consists of two expressions, real and imaginary parts as shown in Eq. (2).

It is also noted that the imaginary part of the refractive index shows the attenuation K of the wave, which is essentially designed to investigate the energy loss of the radiation. It is related to the absorption coefficient by the Eq. (5).

Using the Boltzmann equation mentioned above, we have calculated the variation of the electrical conductivity as a function of temperature. This calculation is very important to describe the electrical behavior of CdSe,

It has been observed that CdSe in cubic and wurtzite structure has an increasing electrical conductivity while the temperature increases, which means that the number of free electrons increases. Our results are in agreement with the experimental results (Suresh and Arunseshan 2014). This conductivity is mainly due to the presence of selenium vacancies as is reported by several researchers. Therefore, we can conclude that CdSe can be exploited as a semiconductor in photovoltaic applications, the conductivity and transmittance which reaches 80 % are significant parameters that allow us to consider this material as a candidate in solar cell applications.

## Conclusion

We have calculated the electronic, optical and electrical properties of CdSe in different phases, cubic and wurtzite model with different approximations. Using Boltztrap equations and FP-LAPW method with the generalized gradient approximation (GGA), local density approximation and mBJ approach. The calculations show that the cubic structure is isotope while for wurtzite structure the propagation of radiation hν is different in xx and zz directions.

The decreases of absorption coefficient in the visible light, a stable transmittance which reach 80 % in the visible light range beyond 400 nm were showed. We have investigated also that with increasing temperature, the electrical conductivity increases. The optical absorption is significant in the ultraviolet field. We have shown favorable results between calculations and the existing experimental data, these results confirm the quality that can present CdSe to be used as suitable material in optoelectronic and photovoltaic applications.

## Declarations

### Authors’ contributions

All authors have contributed equally to this work. All authors work in our laboratory and they have contributed to this work. All authors read and approved the final manuscript.

### Acknowledgements

We would like to thank Mr. P. Blaha and Mr. K. Schwarz for the WIEN2k code that we used for this study. We would like also to thank Katarzyna Kula for the correction that she made to our manuscript.

### Compliance with ethical guidelines

**Competing interests** The authors declare that they have no competing interests.

**Open Access**This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.

## Authors’ Affiliations

## References

- Abbassi A, Ez-Zahraouy H, Benyoussef A (2015) First principles study on the electronic and optical properties of Al and Si- doped ZnO with GGA and mBJ approximations. Opt Quant Electron 47:1869–1880View ArticleGoogle Scholar
- Akinci Ö, Gürel HH, Ünlü H (2009) Semi-empirical tight binding modelling of CdSTe/CdTe, ZnSSe/ZnSe and ZnSSe/CdSe heterostructures. Thin Solid Films 517:2431–2437View ArticleGoogle Scholar
- Beaulac R, Paul Archer I, Stefan Ochsenbein T, Daniel Gamelin R (2008) Mn
^{2+}doped CdSe quantum dots: new inorganic materials for spin-electronics and spin-photonics. Adv Funct Mater 18:3873–3891View ArticleGoogle Scholar - Blaha P, Schwarz K (2006) WIEN2k. Vienna University of Technology, AustriaGoogle Scholar
- Blaha P, Schwarz K, Madsen GKH, Kvasnicka D, Luitz J (2011) WIEN2k an augmented plane wave + local orbitals program for calculating crystal properties; Karlheinz Schwarz, Techn. Universität Wien, AustriaGoogle Scholar
- Fuentes-Hernandez C, Suh DJ, Bernard Kippelen, Marder Seth R (2004) High-performance photorefractive polymers sensitized by cadmium selenide nanoparticles. Appl Phys Lett 85:534–536View ArticleGoogle Scholar
- Kale RB, Lokhande CD (2005) Band gap shift, structural characterization and phase transformation of CdSe thin films from nanocrystalline cubic to nanorod hexagonal on air annealing. Semicond Sci Technol 20:1–9View ArticleGoogle Scholar
- Karl W, Frese Jr (1982) A high efficiency singlecrystal CdSe photoelectrochemical solar cell and an associated loss mechanism. Appl Phys Lett 40:275–277View ArticleGoogle Scholar
- Klude M, Passow T, Heinke H, Hommel D (2002) Electro-optical characterization of CdSe quantum dot laser diodes. Phys Status Solidi B 229:1029–1032View ArticleGoogle Scholar
- Madsen GKH, Singh DJ (2006) BoltzTraP. A code for calculating band-structure dependent quantities. Comput Phys Commun 175:67–71View ArticleGoogle Scholar
- Marcel Bruchez Jr, Moronne M, Gin P, Weiss S, Paul Alivisatos A (1998) Semiconductor nanocrystals as fluorescent biological level. Science 281:2013–2016View ArticleGoogle Scholar
- Matsumura N, Endo H, Saraie J (2002) Fabrication of ZnSe diodes with CdSe quantum-dot layers by molecular beam epitaxy. Phys Status Solidi B 229:1039–1042View ArticleGoogle Scholar
- Merad AE, Kanoun MB, Merad G, Cibert J, Aourag H (2005) Full-potential investigation of the electronic and optical properties of stressed CdTe and ZnTe. Mater Chem Phys 92:333–339View ArticleGoogle Scholar
- Merad AE, Kanoun MB, Goumri-Said S (2006) Ab initio study of electronic structures and magnetism in ZnMnTe and CdMnTe diluted magnetic semiconductors. J Magn Magn Mater 302:536–542View ArticleGoogle Scholar
- Murray CB, Norris DJ, Bawendi MG (1993) Synthesis and characterization of nearly monodisperse CdE (E=S, Se, Te) semiconductor nanocrystallites. J Am Chem Soc 115:8706–87015View ArticleGoogle Scholar
- Ninomiya S, Adachi S (1995) Optical properties of wurtzite CdS. J Appl Phys 78:1183–1190View ArticleGoogle Scholar
- Perdew JP, Burke K, Ernzerhof M (1996) Generalized gradient approximation made simple. Phys Rev Lett 77:3865–3868View ArticleGoogle Scholar
- Slater JC (1951) Simplification of the Hartree Fock method. Phys Rev 81:385–390View ArticleGoogle Scholar
- Suresh S, Arunseshan C (2014) Dielectric properties of cadmium selenide (CdSe) nanoparticles synthesized by solvothermal method. Appl Nanosci 4:179–184View ArticleGoogle Scholar
- Uthana S, Reddy PJ (1981) Electrical properties of CdSe thin films. J Phys Status Solidi A 65:K113–K115View ArticleGoogle Scholar
- Ziman JM (2001) Electrons and phonons. Oxford University Press, New YorkView ArticleGoogle Scholar